The Use of Fly Ash and Lime Sludge as Partial Replacement
of Cement in Mortar
, V. Gayathri
Department of Civil & Environmental Engineering, ITM University, Gurgaon, Haryana, India.
Received 05 July 2013; received in revised form 19 October 2013; accepted 28 November 2013
The increased demand of drinking water and power has led huge generation of water treatment plant residue i.e. sludge and the thermal power plant by-product such as fly ash. Large quantities of sludge and fly ash are produced in India and disposed off by landfilling or dumping in and around sites. In this study fly ash and water softening sludge (lime sludge) has been utilized in mortar. Two types of mortar (type I and II) with four binder combinations have been tried. Binder I consists of 70% fly ash (FA) and 30% lime sludge (LS) , 0 % gypsum (G), binder II is 70% FA, 30% LS and 1% G, binder III is 50% FA, 30% LS and 20% cement and the binder IV is 40% FA, 40% LS with 20% cement. The effect of various combinations on strength has been discussed here. This paper outlines the composition of the composite material, method of preparation of mortar specimen, testing procedure and salient results thereof.
Keywords: Fly ash, lime sludge, mortar
The creation of non-decaying waste materials, combined with a growing consumer population has resulted in a waste disposal crisis leading to an economic and environmental problem. These wastes that produced today will remain in the environment for hundreds, perhaps thousands of years. The magnitude of environmental problems like air, surface and ground water pollution and economic problem like landfilling maintenance cost, etc., is very high for both wastes. This rapidly increasing waste stream remains a significant environmental issue and needs to manage in an economic and environmentally sustainable manner. India also faces this crisis to a large extent. One solution to this crisis lies in recycling waste into useful products to replace the natural/commercial products wherever possible which will reduce the economic and environmental problem of waste disposal and also reduce the depletion of natural resources. Large quantities of drinking water treatment plant sludge are produced in India and across globe and disposed off by landfilling. Space limitations on existing landfill sites and problem of waste stabilization have prompted investigations into alternative reuse techniques and disposal routes for sludge. The best practical way of recycling these wastes is to use in civil engineering constructions since bulk quantities of materials are used in a short time in civil engineering constructions.
The demand for electric power and drinking water had risen tremendously in India because of the industrialization and rapid economic growth. This has resulted in setting up of large number of thermal power plants for the generation of electricity
*Corresponding author. E-mail address: firstname.lastname@example.org, email@example.com
and water purification plants for supplying drinking water. In India, the thermal power generation constitutes 73% of the total power generation installed capacity. Out of which nearly 90% is coal based power generation. The high ash content (30-50%) of Indian coal is a contributing factor for the huge production of fly ash. Fly ash (FA) generation in India was 112 Mt during 2005 and it is expected to hike between 150 and 170 Mt per year by the end of 2012 . Formation of FA depends on the ash content of coal and Indian coal used in power plants generally has very high ash content (35–45%) and is of lower quality . As a consequence, a large amount of FA is generated in thermal power plants, and is disposed off in unmanaged landfills, lagoons and ponds. FA disposal in an unscientific way affects the local ecosystems due to the heavy metal pollution through erosion and leachate generation. The scenario with respect to fly ash management has undergone considerable improvement over the past few years. Due to increasing dependence on coal as a major resource for energy production and growing environmental concern due to the haphazard of FA disposal, it has become imperative exploring viable avenues for FA management. Hence, the thrust of this discussion was to review the existing FA management options in India and recommend strategies for minimizing the problems related to FA disposal and encouraging its effective utilization.
Lime sludge is generated from paper, acetylene, sugar, fertilizer, sodium chromate, soda ash industries, and water softening plants. Approximately 4.5 million tons of sludge in total is generated annually from these indu stries. The study has revealed that sludge from paper industry can be utilized up to 74 percent (dry basis) as a component of raw mix for the manufacture of cement clinker. In addition to it around 30 percent (dry basis) lime sludge can also be utilized fo r the manufacture of masonry cement. Due to the presence of higher quantities of deleterious constituents in carbide sludge, it can be used up to 30 percent whereas level of utilization for other sludge could reach to only 10 percent in the manufacture of cement clinker .
While considerable development has been made in utilization of fly ash which was just 3% in 1994, increased to 13% in 2002, and reached almost 50% in 2011, the water treatment plant sludge need more attention for their reuse. Continuous efforts are under way to find applications where fly ash can be used effectively in bulk quantities in several civil engineering applications for example using as a fill material [4, 14, 15], as a lightweight aggregate [3, 6, 17, 29, 30], as a subbase material [5, 12, 23, 33, 21] for the manufacture of clay flooring and terracing tiles [7, 35] as an absorbent material [13, 16], as a binder material in concrete technology [2, 11, 27], and as a volume replacement and self-compacting material for increasing the workability of concrete [19, 20, 26, 34, 36, 38]. Strength development in fly ash is critical in most applications, but it varies considerably depending on several parameters.
However, unlike the case of fly ash which has several papers and reviews on its beneficial reuse already published, it appears beneficial reuses of lime sludge is lacking for now. Few constructive attempts and research works have been made particularly in recent years to reuse waterworks sludge in many beneficial ways. Utilization of lime sludge in India is very limited, the incorporation of lime sludge for productivity enhancement of lime kilns was tried and found feasible  and incorporation of lime sludge in cement manufacturing was discussed in CPCB report .
2.1. Fly ash
Fly ash used is collected from Badarpur thermal power plant, Delhi. The fly ash was collected from the electrostatic precipitators and stored in air tight bins. Morphological characteristics were determined for the fly ash. The chemical composition for the fly ash has been referred from literature.
2.2. Lime sludge
Sludge used in this study is collected from water treatment plant, Delhi, India with installed capacity of 4.5 million liters per day (MLD) and producing about 4-5 ton of sludge daily. During the process of producing potable water, some commercial products are added to raw water in order to assure its quality for human consumption. In the present study calcium hydroxide, poly aluminum chloride (PAC) and a flocculating agent were added to treat the water. The flocs produced during coagulation and flocculation treatment is settled in the clarifier. The sludge is collected from the bottom of the clarifier and stored in the sump tank. A centrifuge thicker is used to remove the water content of the sludge and make it dry. The sludge collected after centrifuge thickening process was in dry state and stored properly in air tight containers.
2.3. Cement and sand
An ordinary Portland cement of 43 grades has been used in the present work. The river bed sand passing through sieve size 4.75 mm has been used in the study.
Analytical grade calcium sulphate dihydrate (gypsum) CaSO4.2H2O has been used.
Characteristics of Fly Ash and Lime Sludge
3.1. Morphological characteristics
The morphological characteristics of fly ash and lime sludge were studied by scanning electron microscopic technique. Zeiss EVO series scanning electron microscope model EVO 50 was used to examine the morphology of the materials. Figure 1 (a) and (b) show the scanning electron micrographs of fly ash and sludge respectively at 5000 times magnification. The fly ash particles are spherical in shape and have a wide range of particle size or diameter while the sludge particles are irregular in shape and show the agglomerated structure.
3.2. Chemical composition
The chemical composition of Indian lime sludge and fly ash referred from literature is presented in table 1. It shows that generally the fly ash is rich in silica (SiO2) and alumina (Al2O3), the lime sludge contains a good amount of calcium oxide (CaO). Hence this combination can replace cement which generally contains large amount of CaO and less concentration of silica and alumina.
Table 1 Chemical composition of fly ash and lime sludge in India
Mineral SiO2 Al2O3 Fe2O3 CaO MgO LOI SO3 Na2O
Fly ash1 38-63 27-44 3.3-6.4 0.2-8 0.01-0.5 0.2-3.4 --- ---
Lime sludge2 2-8 0.8-5 0.8-2.5 35-70 0.2-10 20-50 0.2-9 0.8-2.0
Source: 1Pandian, 2004 2CPCB, 2007
4.1. Mix preparation
The fly ash and ordinary Portland cement was sieved and portion retained on 90 micron was used. The sludge was oven dried for about 16-18 hours at 60oC and the lumps were broken gently using the pestel. It was sieved through 150 micron sieve and portion retained on 90 micron sieve was used. Two sets of mortar mix (type I and type II) were prepared, each set with two different types of binders. Type I mortar is cement less mortar, where 100% cement is replaced with a combination of fly ash and lime sludge with 0 & 1% of gypsum. Type II mortar consists of 20% cement content, fly ash and lime sludge. All the sets of mortar were prepared with 1:3 binder-to-sand ratio. In this paper, the mixes are designated by a common coding system consisting of three alphabets, namely ‘FA’ for fly ash, ‘LS’ for lime sludge, ‘C’ for cement and ‘G’ for gypsum. The variables
used are presented in table 2.
Table 2 Variables used in the study
Binder name FA (%) LS (%) C (%) G (%)
Type I - without cement
Binder I 70 30 0 0
Binder II 70 30 0 1
Type II - with cement content
Binder III 50 30 20 0
Binder IV 40 40 20 0
4.2. Consistency test
To determine the water content for the mortar mix, consistency test for all the three binder combination was performed. The consistency was determined as per IS: 4031 (Part 4)-1988. 200 g of binder materials were weighed and mix with 35, 38 and 40 % of water and check for penetration of plunger from bottom. At 40% of water content, the penetration was within the range of 5-7 mm. Hence optimum water content was 40% and standard consistency (P) was determined as 13%.
4.3. Specimen preparation
4.4. Method of curing
It was observed that certain specimens could not be taken out from the mould after 24 h indicating that the rate of strength gain was slower in first 2 days. To make the curing uniform, all the specimens were demoulded after about 48 hours and were kept in humidity chamber for moist curing. The humidity chamber was maintained at 95% relative humidity and 25oC temperature. The curing was continued till the respective specimens were tested after 3, 7 and 28 days for compressive strength.
4.5. Compressive strength test
For each binder combination three identical specimens were tested. The samples were tested on a universal testing machine. As an acceptance criterion, the specimen, whose individual strength deviated by more than 10% from an average strength of the three identical specimens, was rejected. The tests were conducted on all combinations of fly ash – lime sludge – cement and gypsum.
Results and Discussion
5.1. Type I mortar with 0% cement (cement less)
Fig. 2 Compressive strength versus curing period for type I mortar
with fly ash in mortar mix without adding any cement to it. After extensive studies the binder II (with gypsum) can be successfully used in various applications.
Table 3 Percent increase in strength with curing period
Curing period Percent increase
Binder I (0% gypsum)
Binder II (1% gypsum)
Table 4 Percent increase in strength on gypsum addition
Curing period Percent increase
5.2. Type II mortar with 20% cement
Under this section, 20% of cement was added along with fly ash and lime sludge. Binders III & IV, namely 50FA:30LS:20C and 40FA:40LS:20C were prepared. In binder III, FA content is more (50%) and LS is less (30%) whereas in binder IV, the FA content was decreased from 50 to 40% and LS content increased from 30 to 40%, the cement content is kept constant in both the binders. Figure 3 shows the strength of both the binders. It is observed that the strength gain is more in binder IV (40FA:40LS:20C) than binder III (50FA:30LS:20C). The strength increases with increase in lime sludge content (from 30 to 40%) and subsequent reduction in fly ash content (from 50 to 40%). The reason may be due to the presence of calcium oxide (CaO) in lime sludge which is responsible for strength gain. Hence sludge addition shows strength gain. The highest strength of 14 N/mm2 was observed for binder IV. The percent increase in strength for binder IV as compared to binder III is given in table 5.
Fig. 3 Compressive strength versus curing period for type II mortar
Table 5 Percent increase in strength for binder IV as compared to binder III
Curing period Percent increase
Beneficial utilization of fly ash and lime sludge in mortar mix presents an opportunity to achieve sustainable utilization of natural and/or conventional resources. The four binders discussed here can be gainfully exploited as the building materials in construction. Continue refinement of optimum content, long term strength, durability studies, and leachate analysis of the composite could provide a way to effectively utilize these waste materials as an economic and sustainable development strategy.
The study brings forth the following conclusions:
(1) This work brings forth the compatibility of two potential industrial by-products namely fly ash and lime sludge in mortar mix.
(2) The large amount of silica and alumina available in fly ash and rich content of calcium oxide in lime sludge, make them compatible with each other and can replace cement also.
(3) The strength was increased continuously with curing period.
(4) The addition of gypsum showed positive effect on strength due to accelerated pozzolanic reaction. For type I mortar, the highest strength of 6 N/mm2 was observed for binder II (1% gypsum) after 28 days curing period.
(5) By increasing the content of LS and subsequent decrease of FA content under type II mortar showed increased strength of binder IV as compared to binder III. The maximum strength achieved after 28 days curing for type II mortar was 14 N/mm2 (binder IV).
 G. Ambarish and D. Utpal, “Bearing ratio of reinforced fly ash overlying soft soil and defomation modulus of fly ash,” Geotextiles and Geomembranes, vol. 27, no. 4, pp. 313-320, 2009.
 N. M. Aneta, “Water-binder ratio influence on de-icing salt scaling of fly ash concrete,” Procedia Engineering, vol. 57, pp. 823-829, 2013.
 S. Angelo, O. Robert, G. Terry, and P. Jan, “Artificial lightweight aggregates as utilization for future ashes – A case study,” Waste Management, vol. 32, no. 1, pp. 144-152, 2012
 A. Das, C. Jayashree, and B.V.S. Viswanadham, “Effect of randomly distributed geofibers on the piping behaviour of embankments constructed with fly ash as a fill material,” Geotextiles and Geomembranes, vol. 27, no. 5, pp. 341-349, 2007.
 A. Senol, T. B. Edil, B. S. Md.Sazzad, H. A. Acosta, and C. H. Benson, “Soft subgrades stabilization by using various fly ashes,” Resources, Conservation and Recycling, vol. 46, no. 4, pp. 365-376, 2006.
 S. B. Shafique, T. B. Edil, C. H. Benson, and A. Senol, “Incorporating a fly ash stabilized layer into pavement design,” Proceedings of the ICE - Geotechnical Engineering, vol. 157, no. 4, pp. 239–249, 2004.
 E. Bou, M. F. Quereda, D. Lever, A. R. Boccaccini, and C. R. Cheeseman, “Production of pulverised fuel ash tiles using conventional ceramic production processes,” Advances in Applied Ceramics, vol. 108, no. 1, pp. 44-49, 2009.
 K. C. Cameron, H. J. Di, and R. G. McLaren, “Is soil an appropriate dumping ground for our wastes?” Australian Journal of Soil Research, vol. 35, no. 5, pp. 995-1035, 1997.
 CPCB,“Assessment of utilization of industrial solid wastes in cement manufacturing,” Central Pollution Control Board, New Delhi,2007.
 CPCB, “Fly ash generation at coal/lignite based thermal power stations and its utilization in the country for 1st half of the year 2011-2012,” Central Electricity Authority, 2011.
 D. Ravikumar, S. Peethamparan, and N. Neithalath, “Structure and strength of NaOH activated concretes containing fly ash or GGBFS as the sole binder,” Cement and Concrete Composites, vol. 32, no. 6, pp. 399-410, 2010.
 V. Hequet, P. Ricou, I. Lecuyer, and P. L. Cloirec, “Removal of Cu+2 and Zn+2 in aqueous solution by sorption onto mixed fly ash,” Fuel, vol. 80, no. 6, pp. 851-856, 2001.
 H. Y. Jo, S. H. Min, T. Y. Lee, H.S. Ahn, S. H. Lee, and J. K. Hong, “Environmental feasibility of using coal ash as a fill material to raise the ground level,” Journal of Hazardous Materials, vol. 154, no. 1-3, pp. 933-945, 15 June 2008.  S. Horiuchi, M. Kawaguchi, and K. Yasuhara “Effective use of fly ash slurry as fill material,” Journal of Hazardous
Materials, vol. 76, pp. 301-337, 2000.
 I. J. Alinnor, “Adsorption of heavy metals from aqueous solutions by fly ash,” Fuel, vol. 86, no. 5-6, pp. 853-857, 2007  I. Kourti and C. R. Cheeseman, “Properties and microstructure oflight weight aggregate produced from lignite coal fly ash
and recycled glass,” Resources, Conservation and Recycling, vol. 54, no. 11, pp. 769-775, 2010.  IS: 4031 (part 4) – 1988, Bureau of Indian Standards, New Delhi.
 C. Jaturapitakkul, K. Kiattikomol, V. Sata, and T. Leekeeratikul, “Use of ground coarse fly ash as a replacement of silica fume in producing high strength concrete,” Cement and Concrete Composites, vol. 34, 549-555, 2004.
 J. Cuenca, J. Rodriguez, M. Martin-Morales, Z. Sánchez-Roldán, and M. Zamorano, “Effects of olive residue biomass fly ash as filler in self-compacting concrete,” Construction and Building Materials, vol. 40, pp. 702-709, 2013.
 J. T. Shahu, S. Patel, and A. Senapati, “Engineering properties of copper slag-fly ash-dolime mix and its utilization in base course of flexible pavements,” Journal of Materials in Civil Engineering, 2012.
 J. W. van de Lindt, J.A.H. Carraro, P. R. Heyliger, and C. Choi, “Application and feasibility of coal fly ash and scrap tire fiber as wood wall insulation supplements in residential buildings,” Resources, Conservation and Recycling, vol. 52, no. 10, pp. 1235-1240, 2008.
 B. Leelavathamma, K. M. Mini, and N. S. Pandian, “California bearing ratio behavior of soil-stabilized class F fly ash systems,” Journal of Testing and Evaluation, vol. 33, no. 6, pp. 406–410, 2005.
 R. Mathur, S. Chand, and T. Tezuka, “Optimal use of coal for the power generation in India,” Energy Policy, vol. 31, pp. 319-331, 2003.
 Ministry of Environment and Forests, Ministry of Environment and Forests (MOEF) notification, Fly ash notification 2007, New Delhi, 3rd Apr. 2007.
 S. Mustafa, O. Y. Ismail, and T. Mustafa, “Transport and mechanical properties of self-consolidating concrete with high volume fly ash,” Cement and Concrete Composites, vol. 31, pp. 99-106, 2009.
 M. Nattapong, J. Chai, N. Charin, and S. Vanchai, “Effects of binder and CaCl2 contents on the strength of calcium carbide residue-fly ash concrete,” Cement and Concrete Composites, vol. 33, no. 3, pp. 436-443, 2011.
 NCC&BM, “Report on Utilization of lime sludge for value added products and productivity enhancement of lime kilns,” National Council for Cement and Building Material, New Delhi, 2003.
 N. U. Kockal and T. Ozturan, “Effects of lightweight fly ash aggregates properties on the behaviour of lightweight concretes,” Journal of Hazardous Materials, vol. 179, no. 1-3, pp. 954-965, 2010.
 N. U. Kockal and T. Ozturan, “Characteristics of lightweight fly ash aggregates produced with different binders and heat treatments,” Cement and Concrete Composites, vol. 33, no. 1, pp. 61-67, 2011.
 N. S. Pandian, “Fly ash characterization with reference to geotechnical applications,” Journal of Indian of Institute of Science, vol. 84, pp. 189-216, 2004.
 R. A. Aguilar, O. B. Diaz, and J.I.E. Garcia, “Lightweight concretes of activated metakaolin- fly ash binders, with blast furnace slag aggregates,” Construction and Building Materials, vol. 24, no. 7, pp. 1166-1175, 2010.
 B. S. Sazzad, K. Rahman, M. Yaykiran, and I. Azfar, “The long-term performance of two fly ash stabilized fine-grained soil subbases,” Resources, Conservation and Recycling, vol. 54, no. 10, pp. 666-672, 2010.
 R. Siddique, “Effect of fine aggregate replacement with class F fly ash on the mechanical properties of concrete,” Cement and Concrete Research, vol. 33, pp. 539-547, 2003.
 S. Ramesh, “Appraisal of vernacular building materials and alternative technologies for roofing and terracing options of embodied energy in buildings,” Energy Procedia, vol. 14, pp. 1843-1848, 2012.
 S. Tsimas, and A. M. Tsima, “High-calcium fly ash as a fourth constituent in concrete: Problems, solutions and perspectives,” Cement & Concrete Composites, vol. 27, no. 2, pp. 231-237, 2005.
 L. W. Titshall and J. C. Hughes, “Characterization of some South African water treatment residues and implications for land application”. Water SA, vol. 31, no. 3, pp. 299-307, 2005.